#------------------------------------------------------------------------------
#$Date: 2016-03-23 01:35:19 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179147 $
#$URL: svn://www.crystallography.net/cod/cif/4/31/08/4310826.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4310826
loop_
_publ_author_name
'Ulrich Kortz'
'Saritha Nellutla'
'Ashley C. Stowe'
'Naresh S. Dalal'
'Urs Rauwald'
'Welbeck Danquah'
'Didier Ravot'
_publ_section_title
;
 Sandwich-type Germanotungstates: Structure and Magnetic Properties of the
 Dimeric Polyoxoanions [M₄(H₂O)₂(GeW₉O₃₄)₂]¹²⁻ (M = Mn²⁺,
 Cu²⁺, Zn²⁺, Cd²⁺)
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2308
_journal_page_last               2317
_journal_paper_doi               10.1021/ic0354421
_journal_volume                  43
_journal_year                    2004
_chemical_formula_sum            'Ge2 H68 Na12 O102 W18 Zn4'
_chemical_formula_weight         5692.58
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                97.828(6)
_cell_angle_beta                 106.169(6)
_cell_angle_gamma                112.113(5)
_cell_formula_units_Z            1
_cell_length_a                   11.589(3)
_cell_length_b                   12.811(3)
_cell_length_c                   17.221(4)
_cell_measurement_reflns_used    5987
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      28.20
_cell_measurement_theta_min      2.27
_cell_volume                     2189.9(9)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.955
_diffrn_measured_fraction_theta_max 0.955
_diffrn_measurement_device_type  'SMART CCD area detector'
_diffrn_measurement_method       'omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'normal-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0568
_diffrn_reflns_av_sigmaI/netI    0.0743
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            25220
_diffrn_reflns_theta_full        28.37
_diffrn_reflns_theta_max         28.37
_diffrn_reflns_theta_min         1.28
_diffrn_standards_decay_%        0
_exptl_absorpt_coefficient_mu    25.468
_exptl_absorpt_correction_T_max  0.3558
_exptl_absorpt_correction_T_min  0.1566
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    4.264
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             2464
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.06
_refine_diff_density_max         4.439
_refine_diff_density_min         -2.314
_refine_diff_density_rms         0.504
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.029
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     394
_refine_ls_number_reflns         10478
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.029
_refine_ls_R_factor_all          0.0718
_refine_ls_R_factor_gt           0.0450
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0445P)²+38.8499P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0988
_refine_ls_wR_factor_ref         0.1177
_reflns_number_gt                7794
_reflns_number_total             10478
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic0354421si20031215_053049_4.cif
_cod_data_source_block           u122abs
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_database_code               4310826
loop_
_publ_contact_author_name
_publ_contact_author_address
_publ_contact_author_email
_publ_contact_author_fax
_publ_contact_author_phone
'Ulrich KORTZ'
; 
International University Bremen
School of Engineering and Science
P.O. Box 750 561
28725 Bremen
Germany
;
u.kortz@iu-bremen.de '+49-421-200 3229' '+49-421-200 3235'
'Naresh S. Dalal'
; 
Department of Chemistry and Biochemistry
Florida State University and
National High Magnetic Field Laboratory
Tallahassee, FL 32306-4390 
USA 
;
dalal@chemmail.chem.fsu.edu '+1-850-644 3398' '+1-850-644 8281'
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.10813(5) 0.61181(5) 0.40080(3) 0.01202(12) Uani 1 1 d . . .
W2 W 0.41349(5) 0.65593(5) 0.35002(3) 0.01191(12) Uani 1 1 d . . .
W3 W 0.15722(5) 0.35224(5) 0.31530(3) 0.01142(12) Uani 1 1 d . . .
W4 W 0.03903(5) 0.77279(5) 0.26896(4) 0.01246(12) Uani 1 1 d . . .
W5 W 0.33994(5) 0.81655(5) 0.21813(4) 0.01206(12) Uani 1 1 d . . .
W6 W 0.38800(5) 0.58628(5) 0.14523(3) 0.01077(12) Uani 1 1 d . . .
W7 W 0.13032(5) 0.28506(5) 0.11169(3) 0.01008(12) Uani 1 1 d . . .
W8 W -0.14553(5) 0.24695(5) 0.15542(3) 0.01121(12) Uani 1 1 d . . .
W9 W -0.19151(5) 0.50441(5) 0.24115(3) 0.01204(12) Uani 1 1 d . . .
Ge1 Ge 0.08558(13) 0.53553(12) 0.18100(9) 0.0103(3) Uani 1 1 d . . .
Zn1 Zn -0.15125(15) 0.58778(14) 0.05670(10) 0.0117(3) Uani 1 1 d . . .
Zn2 Zn 0.11087(15) 0.62986(13) 0.01507(10) 0.0117(3) Uani 1 1 d . . .
Na1 Na 0.4500(6) 0.4102(5) 0.2718(4) 0.0239(13) Uani 1 1 d . . .
Na2 Na 0.4720(7) 0.1565(6) 0.3093(4) 0.0316(15) Uani 1 1 d . . .
Na3 Na -0.1311(6) -0.0116(5) 0.0258(4) 0.0234(13) Uani 1 1 d . . .
Na4 Na 0.7793(6) 0.7441(6) 0.4787(4) 0.0279(14) Uani 1 1 d . . .
Na5 Na -0.1110(11) 0.3239(10) 0.3684(7) 0.018(2) Uani 0.50 1 d P . .
Na6 Na -0.3249(14) 0.0420(13) 0.2582(10) 0.042(4) Uani 0.50 1 d P . .
Na7 Na -0.5000 0.0000 0.0000 0.042(3) Uani 1 2 d S . .
Na8 Na -0.1156(14) -0.0082(13) 0.4269(9) 0.038(3) Uani 0.50 1 d P . .
O1GE O 0.0277(9) 0.5892(8) 0.2537(6) 0.0118(19) Uiso 1 1 d . . .
O1T O 0.1487(10) 0.6344(9) 0.5068(6) 0.020(2) Uiso 1 1 d . . .
O1ZW O -0.2978(9) 0.6496(8) 0.0412(6) 0.017(2) Uiso 1 1 d . . .
O2GE O 0.2579(9) 0.6231(8) 0.2156(6) 0.0118(19) Uiso 1 1 d . . .
O2T O 0.5461(9) 0.6937(8) 0.4407(6) 0.016(2) Uiso 1 1 d . . .
O3GE O 0.0647(8) 0.3946(8) 0.1895(6) 0.0101(18) Uiso 1 1 d . . .
O3T O 0.2132(9) 0.2953(8) 0.3938(6) 0.016(2) Uiso 1 1 d . . .
O4GE O -0.0003(9) 0.5302(8) 0.0796(6) 0.0120(19) Uiso 1 1 d . . .
O4T O 0.0422(10) 0.9107(9) 0.3027(6) 0.020(2) Uiso 1 1 d . . .
O4ZN O -0.0248(9) 0.7384(8) 0.1589(6) 0.014(2) Uiso 1 1 d . . .
O5T O 0.4356(9) 0.9656(8) 0.2340(6) 0.016(2) Uiso 1 1 d . . .
O5ZN O 0.2200(9) 0.7751(8) 0.1161(6) 0.014(2) Uiso 1 1 d . . .
O6T O 0.5110(9) 0.5778(9) 0.1122(6) 0.018(2) Uiso 1 1 d . . .
O6ZN O 0.2553(9) 0.5609(8) 0.0501(6) 0.016(2) Uiso 1 1 d . . .
O7A O 0.0590(9) 0.3290(8) 0.0218(6) 0.015(2) Uiso 1 1 d . . .
O7T O 0.1815(9) 0.1875(9) 0.0714(6) 0.018(2) Uiso 1 1 d . . .
O8A O -0.1925(9) 0.2891(8) 0.0639(6) 0.016(2) Uiso 1 1 d . . .
O8T O -0.2833(9) 0.1198(9) 0.1429(6) 0.019(2) Uiso 1 1 d . . .
O9T O -0.3418(9) 0.4605(8) 0.2560(6) 0.017(2) Uiso 1 1 d . . .
O9ZN O -0.2336(9) 0.4987(8) 0.1326(6) 0.016(2) Uiso 1 1 d . . .
O12 O 0.2818(9) 0.6666(8) 0.3929(6) 0.015(2) Uiso 1 1 d . . .
O13 O 0.1092(9) 0.4595(8) 0.3725(6) 0.015(2) Uiso 1 1 d . . .
O14 O 0.1067(9) 0.7535(8) 0.3895(6) 0.0133(19) Uiso 1 1 d . . .
O19 O -0.0802(9) 0.5323(8) 0.3631(6) 0.017(2) Uiso 1 1 d . . .
O23 O 0.3159(9) 0.4906(8) 0.3324(6) 0.0125(19) Uiso 1 1 d . . .
O25 O 0.4509(9) 0.8024(8) 0.3299(6) 0.0127(19) Uiso 1 1 d . . .
O26 O 0.4842(9) 0.6145(8) 0.2693(6) 0.015(2) Uiso 1 1 d . . .
O37 O 0.1998(8) 0.2781(7) 0.2319(6) 0.0094(18) Uiso 1 1 d . . .
O38 O -0.0239(9) 0.2440(8) 0.2667(6) 0.016(2) Uiso 1 1 d . . .
O45 O 0.2208(9) 0.8200(8) 0.2757(6) 0.0133(19) Uiso 1 1 d . . .
O49 O -0.1312(9) 0.6742(8) 0.2740(6) 0.018(2) Uiso 1 1 d . . .
O56 O 0.4466(9) 0.7522(8) 0.1741(6) 0.0124(19) Uiso 1 1 d . . .
O67 O 0.2975(9) 0.4276(8) 0.1489(6) 0.0130(19) Uiso 1 1 d . . .
O78 O -0.0401(9) 0.1803(8) 0.1105(6) 0.014(2) Uiso 1 1 d . . .
O89 O -0.1736(8) 0.3584(8) 0.2244(6) 0.0106(18) Uiso 1 1 d . . .
O1W O -0.3291(10) 0.0114(9) -0.0561(7) 0.026(2) Uiso 1 1 d . . .
O2W O 0.7560(10) 0.5462(9) 0.4533(7) 0.023(2) Uiso 1 1 d . . .
O3W O 1.0184(14) 0.7974(12) 0.5268(9) 0.049(4) Uiso 1 1 d . . .
O4W O -0.0585(11) 0.0556(10) -0.0860(7) 0.028(3) Uiso 1 1 d . . .
O5W O -0.4972(11) 0.3236(10) 0.0689(7) 0.030(3) Uiso 1 1 d . . .
O6W O -0.5118(12) 0.1528(11) -0.0484(8) 0.039(3) Uiso 1 1 d . . .
O7W O -0.2219(12) -0.1135(11) 0.1162(8) 0.040(3) Uiso 1 1 d . . .
O8W O 0.5110(11) 0.3468(10) 0.3928(7) 0.029(3) Uiso 1 1 d . . .
O9W O 0.4319(11) 0.2205(10) 0.1879(7) 0.027(2) Uiso 1 1 d . . .
O10W O 0.2302(11) 0.0832(10) 0.2521(7) 0.028(3) Uiso 1 1 d . . .
O11W O -0.1150(13) 0.0276(12) 0.2944(8) 0.044(3) Uiso 1 1 d . . .
O12W O 0.7559(11) 0.7842(10) 0.3471(7) 0.027(3) Uiso 1 1 d . . .
O13W O -0.3101(13) -0.0045(12) 0.3886(9) 0.045(3) Uiso 1 1 d . . .
O14W O 0.880(2) 0.964(2) 0.5300(14) 0.027(5) Uiso 0.50 1 d P . .
O15W O 0.383(2) 0.926(2) 0.4626(15) 0.034(6) Uiso 0.50 1 d P . .
O16W O 0.551(2) 0.130(2) 0.4441(16) 0.037(6) Uiso 0.50 1 d P . .
O17W O -0.306(2) 0.1921(18) 0.3187(13) 0.022(5) Uiso 0.50 1 d P . .
O18W O 0.395(2) 0.044(2) 0.4136(16) 0.041(6) Uiso 0.50 1 d P . .
O19W O 0.815(2) 0.933(2) 0.5388(15) 0.033(6) Uiso 0.50 1 d P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1T W1 O14 100.3(4) . . ?
O1T W1 O19 101.0(4) . . ?
O14 W1 O19 93.1(4) . . ?
O1T W1 O12 100.9(4) . . ?
O14 W1 O12 89.1(4) . . ?
O19 W1 O12 157.3(4) . . ?
O1T W1 O13 99.4(4) . . ?
O14 W1 O13 159.7(4) . . ?
O19 W1 O13 87.8(4) . . ?
O12 W1 O13 82.6(4) . . ?
O1T W1 O1GE 171.8(4) . . ?
O14 W1 O1GE 74.6(4) . . ?
O19 W1 O1GE 73.3(4) . . ?
O12 W1 O1GE 85.6(4) . . ?
O13 W1 O1GE 86.3(4) . . ?
O1T W1 Na5 90.4(4) . . ?
O14 W1 Na5 140.1(3) . . ?
O19 W1 Na5 47.1(3) . . ?
O12 W1 Na5 126.6(3) . . ?
O13 W1 Na5 44.0(3) . . ?
O1GE W1 Na5 89.7(3) . . ?
O2T W2 O25 99.9(4) . . ?
O2T W2 O26 100.0(4) . . ?
O25 W2 O26 91.2(4) . . ?
O2T W2 O12 101.6(4) . . ?
O25 W2 O12 90.4(4) . . ?
O26 W2 O12 157.8(4) . . ?
O2T W2 O23 102.6(4) . . ?
O25 W2 O23 157.5(4) . . ?
O26 W2 O23 86.0(4) . . ?
O12 W2 O23 84.1(4) . . ?
O2T W2 O2GE 170.0(4) . . ?
O25 W2 O2GE 73.6(4) . . ?
O26 W2 O2GE 73.1(3) . . ?
O12 W2 O2GE 86.1(4) . . ?
O23 W2 O2GE 84.3(3) . . ?
O2T W2 Na1 90.8(3) . . ?
O25 W2 Na1 135.8(3) . . ?
O26 W2 Na1 44.6(3) . . ?
O12 W2 Na1 129.5(3) . . ?
O23 W2 Na1 45.4(3) . . ?
O2GE W2 Na1 89.0(2) . . ?
O3T W3 O38 100.9(4) . . ?
O3T W3 O37 98.1(4) . . ?
O38 W3 O37 91.8(4) . . ?
O3T W3 O13 101.4(4) . . ?
O38 W3 O13 89.7(4) . . ?
O37 W3 O13 159.8(4) . . ?
O3T W3 O23 101.8(4) . . ?
O38 W3 O23 157.3(4) . . ?
O37 W3 O23 86.7(4) . . ?
O13 W3 O23 84.2(4) . . ?
O3T W3 O3GE 168.9(4) . . ?
O38 W3 O3GE 72.8(3) . . ?
O37 W3 O3GE 73.4(3) . . ?
O13 W3 O3GE 87.9(3) . . ?
O23 W3 O3GE 85.1(3) . . ?
O3T W3 Na5 91.2(4) . . ?
O38 W3 Na5 47.6(4) . . ?
O37 W3 Na5 139.5(3) . . ?
O13 W3 Na5 45.7(3) . . ?
O23 W3 Na5 129.9(3) . . ?
O3GE W3 Na5 90.9(3) . . ?
O3T W3 Na1 89.6(3) . . ?
O38 W3 Na1 137.5(3) . . ?
O37 W3 Na1 45.8(3) . . ?
O13 W3 Na1 128.8(3) . . ?
O23 W3 Na1 44.6(3) . . ?
O3GE W3 Na1 89.4(2) . . ?
Na5 W3 Na1 174.4(2) . . ?
O4ZN W4 O4T 104.5(4) . . ?
O4ZN W4 O45 93.9(4) . . ?
O4T W4 O45 100.4(4) . . ?
O4ZN W4 O49 92.9(4) . . ?
O4T W4 O49 98.8(4) . . ?
O45 W4 O49 157.3(4) . . ?
O4ZN W4 O14 159.9(4) . . ?
O4T W4 O14 95.4(4) . . ?
O45 W4 O14 85.0(4) . . ?
O49 W4 O14 81.3(4) . . ?
O4ZN W4 O1GE 87.0(4) . . ?
O4T W4 O1GE 166.7(4) . . ?
O45 W4 O1GE 85.0(3) . . ?
O49 W4 O1GE 73.7(4) . . ?
O14 W4 O1GE 72.9(3) . . ?
O5T W5 O5ZN 102.9(4) . . ?
O5T W5 O45 101.4(4) . . ?
O5ZN W5 O45 95.2(4) . . ?
O5T W5 O56 99.8(4) . . ?
O5ZN W5 O56 91.2(4) . . ?
O45 W5 O56 155.9(4) . . ?
O5T W5 O25 96.8(4) . . ?
O5ZN W5 O25 160.0(4) . . ?
O45 W5 O25 84.2(4) . . ?
O56 W5 O25 82.0(4) . . ?
O5T W5 O2GE 167.4(4) . . ?
O5ZN W5 O2GE 87.9(4) . . ?
O45 W5 O2GE 83.9(4) . . ?
O56 W5 O2GE 73.1(3) . . ?
O25 W5 O2GE 72.1(3) . . ?
O5T W5 Na6 35.3(4) . 1_665 ?
O5ZN W5 Na6 117.0(4) . 1_665 ?
O45 W5 Na6 127.8(4) . 1_665 ?
O56 W5 Na6 68.0(4) . 1_665 ?
O25 W5 Na6 77.8(3) . 1_665 ?
O2GE W5 Na6 133.3(3) . 1_665 ?
O6T W6 O6ZN 104.3(4) . . ?
O6T W6 O56 100.2(4) . . ?
O6ZN W6 O56 93.6(4) . . ?
O6T W6 O67 100.7(4) . . ?
O6ZN W6 O67 90.6(4) . . ?
O56 W6 O67 157.0(4) . . ?
O6T W6 O26 97.1(4) . . ?
O6ZN W6 O26 158.6(4) . . ?
O56 W6 O26 84.0(4) . . ?
O67 W6 O26 83.8(4) . . ?
O6T W6 O2GE 168.1(4) . . ?
O6ZN W6 O2GE 86.4(4) . . ?
O56 W6 O2GE 73.4(3) . . ?
O67 W6 O2GE 84.3(3) . . ?
O26 W6 O2GE 72.5(3) . . ?
O6T W6 Na1 86.4(3) . . ?
O6ZN W6 Na1 133.7(3) . . ?
O56 W6 Na1 129.4(3) . . ?
O67 W6 Na1 43.1(3) . . ?
O26 W6 Na1 45.4(3) . . ?
O2GE W6 Na1 90.1(2) . . ?
O7T W7 O7A 103.9(4) . . ?
O7T W7 O78 100.8(4) . . ?
O7A W7 O78 93.8(4) . . ?
O7T W7 O67 99.0(4) . . ?
O7A W7 O67 91.4(4) . . ?
O78 W7 O67 157.6(4) . . ?
O7T W7 O37 94.8(4) . . ?
O7A W7 O37 161.1(4) . . ?
O78 W7 O37 84.9(4) . . ?
O67 W7 O37 83.2(4) . . ?
O7T W7 O3GE 166.9(4) . . ?
O7A W7 O3GE 88.4(4) . . ?
O78 W7 O3GE 73.6(4) . . ?
O67 W7 O3GE 84.8(3) . . ?
O37 W7 O3GE 73.1(3) . . ?
O7T W7 Na1 84.8(3) . . ?
O7A W7 Na1 132.9(3) . . ?
O78 W7 Na1 130.6(3) . . ?
O67 W7 Na1 41.6(3) . . ?
O37 W7 Na1 45.7(3) . . ?
O3GE W7 Na1 89.9(2) . . ?
O7T W7 Na3 66.8(3) . . ?
O7A W7 Na3 91.9(3) . . ?
O78 W7 Na3 35.6(3) . . ?
O67 W7 Na3 165.8(3) . . ?
O37 W7 Na3 97.7(3) . . ?
O3GE W7 Na3 109.1(2) . . ?
Na1 W7 Na3 132.50(13) . . ?
O8T W8 O8A 104.3(4) . . ?
O8T W8 O89 100.3(4) . . ?
O8A W8 O89 95.3(4) . . ?
O8T W8 O78 100.4(4) . . ?
O8A W8 O78 90.6(4) . . ?
O89 W8 O78 156.3(4) . . ?
O8T W8 O38 96.5(4) . . ?
O8A W8 O38 158.8(4) . . ?
O89 W8 O38 85.0(4) . . ?
O78 W8 O38 81.4(4) . . ?
O8T W8 O3GE 166.4(4) . . ?
O8A W8 O3GE 87.4(4) . . ?
O89 W8 O3GE 85.4(3) . . ?
O78 W8 O3GE 72.0(3) . . ?
O38 W8 O3GE 71.5(3) . . ?
O8T W8 Na5 87.2(4) . . ?
O8A W8 Na5 139.3(4) . . ?
O89 W8 Na5 43.9(3) . . ?
O78 W8 Na5 126.2(3) . . ?
O38 W8 Na5 44.9(3) . . ?
O3GE W8 Na5 88.4(3) . . ?
O8T W8 Na6 33.2(4) . . ?
O8A W8 Na6 134.8(4) . . ?
O89 W8 Na6 83.9(4) . . ?
O78 W8 Na6 107.9(3) . . ?
O38 W8 Na6 66.3(3) . . ?
O3GE W8 Na6 137.2(3) . . ?
Na5 W8 Na6 56.2(3) . . ?
O9T W9 O9ZN 104.2(4) . . ?
O9T W9 O89 101.6(4) . . ?
O9ZN W9 O89 92.8(4) . . ?
O9T W9 O49 99.0(4) . . ?
O9ZN W9 O49 92.3(4) . . ?
O89 W9 O49 156.8(4) . . ?
O9T W9 O19 95.4(4) . . ?
O9ZN W9 O19 160.4(4) . . ?
O89 W9 O19 84.1(4) . . ?
O49 W9 O19 83.5(4) . . ?
O9T W9 O1GE 166.4(4) . . ?
O9ZN W9 O1GE 87.5(4) . . ?
O89 W9 O1GE 84.5(3) . . ?
O49 W9 O1GE 73.1(4) . . ?
O19 W9 O1GE 72.9(3) . . ?
O9T W9 Na5 88.5(4) . . ?
O9ZN W9 Na5 135.6(4) . . ?
O89 W9 Na5 42.8(3) . . ?
O49 W9 Na5 128.1(3) . . ?
O19 W9 Na5 44.6(3) . . ?
O1GE W9 Na5 87.9(3) . . ?
O4GE Ge1 O2GE 113.8(4) . . ?
O4GE Ge1 O1GE 111.9(4) . . ?
O2GE Ge1 O1GE 106.8(4) . . ?
O4GE Ge1 O3GE 110.8(4) . . ?
O2GE Ge1 O3GE 106.5(4) . . ?
O1GE Ge1 O3GE 106.6(4) . . ?
O9ZN Zn1 O1ZW 86.1(4) . . ?
O9ZN Zn1 O4GE 92.2(4) . . ?
O1ZW Zn1 O4GE 176.7(4) . . ?
O9ZN Zn1 O7A 175.6(4) . 2_565 ?
O1ZW Zn1 O7A 98.1(4) . 2_565 ?
O4GE Zn1 O7A 83.6(3) . 2_565 ?
O9ZN Zn1 O4ZN 91.5(4) . . ?
O1ZW Zn1 O4ZN 87.6(4) . . ?
O4GE Zn1 O4ZN 89.7(4) . . ?
O7A Zn1 O4ZN 89.9(4) 2_565 . ?
O9ZN Zn1 O6ZN 93.6(4) . 2_565 ?
O1ZW Zn1 O6ZN 98.5(4) . 2_565 ?
O4GE Zn1 O6ZN 84.4(4) . 2_565 ?
O7A Zn1 O6ZN 84.6(4) 2_565 2_565 ?
O4ZN Zn1 O6ZN 172.3(4) . 2_565 ?
O9ZN Zn1 Zn2 88.9(3) . 2_565 ?
O1ZW Zn1 Zn2 140.8(3) . 2_565 ?
O4GE Zn1 Zn2 41.8(3) . 2_565 ?
O7A Zn1 Zn2 87.0(3) 2_565 2_565 ?
O4ZN Zn1 Zn2 131.4(3) . 2_565 ?
O6ZN Zn1 Zn2 43.1(2) 2_565 2_565 ?
O8A Zn2 O5ZN 93.7(4) 2_565 . ?
O8A Zn2 O4GE 91.3(4) 2_565 2_565 ?
O5ZN Zn2 O4GE 173.9(4) . 2_565 ?
O8A Zn2 O4GE 171.0(4) 2_565 . ?
O5ZN Zn2 O4GE 94.1(4) . . ?
O4GE Zn2 O4GE 81.2(4) 2_565 . ?
O8A Zn2 O6ZN 93.5(4) 2_565 . ?
O5ZN Zn2 O6ZN 92.6(4) . . ?
O4GE Zn2 O6ZN 83.7(4) 2_565 . ?
O4GE Zn2 O6ZN 90.6(3) . . ?
O8A Zn2 O7A 93.4(4) 2_565 2_565 ?
O5ZN Zn2 O7A 93.5(4) . 2_565 ?
O4GE Zn2 O7A 89.6(4) 2_565 2_565 ?
O4GE Zn2 O7A 81.7(3) . 2_565 ?
O6ZN Zn2 O7A 170.6(4) . 2_565 ?
O8A Zn2 Zn1 88.2(3) 2_565 2_565 ?
O5ZN Zn2 Zn1 135.1(3) . 2_565 ?
O4GE Zn2 Zn1 41.7(2) 2_565 2_565 ?
O4GE Zn2 Zn1 89.4(3) . 2_565 ?
O6ZN Zn2 Zn1 42.6(3) . 2_565 ?
O7A Zn2 Zn1 131.3(3) 2_565 2_565 ?
O9T Na1 O8W 93.9(4) 1_655 . ?
O9T Na1 O67 108.5(4) 1_655 . ?
O8W Na1 O67 156.4(4) . . ?
O9T Na1 O26 86.7(4) 1_655 . ?
O8W Na1 O26 126.0(4) . . ?
O67 Na1 O26 64.4(3) . . ?
O9T Na1 O23 143.7(4) 1_655 . ?
O8W Na1 O23 89.9(4) . . ?
O67 Na1 O23 76.5(3) . . ?
O26 Na1 O23 62.6(3) . . ?
O9T Na1 O9W 74.9(4) 1_655 . ?
O8W Na1 O9W 86.8(4) . . ?
O67 Na1 O9W 91.9(4) . . ?
O26 Na1 O9W 143.7(4) . . ?
O23 Na1 O9W 141.4(4) . . ?
O9T Na1 O37 153.3(4) 1_655 . ?
O8W Na1 O37 93.0(4) . . ?
O67 Na1 O37 63.6(3) . . ?
O26 Na1 O37 109.6(4) . . ?
O23 Na1 O37 61.9(3) . . ?
O9W Na1 O37 79.8(4) . . ?
O9T Na1 W6 89.1(3) 1_655 . ?
O8W Na1 W6 160.8(4) . . ?
O67 Na1 W6 32.5(2) . . ?
O26 Na1 W6 35.1(2) . . ?
O23 Na1 W6 76.7(2) . . ?
O9W Na1 W6 112.3(3) . . ?
O37 Na1 W6 92.7(2) . . ?
O9T Na1 W2 111.9(3) 1_655 . ?
O8W Na1 W2 102.5(3) . . ?
O67 Na1 W2 76.3(3) . . ?
O26 Na1 W2 32.4(2) . . ?
O23 Na1 W2 32.7(2) . . ?
O9W Na1 W2 167.7(3) . . ?
O37 Na1 W2 91.6(3) . . ?
W6 Na1 W2 58.98(10) . . ?
O9T Na1 Na2 85.5(3) 1_655 . ?
O8W Na1 Na2 44.9(3) . . ?
O67 Na1 Na2 127.7(3) . . ?
O26 Na1 Na2 167.4(3) . . ?
O23 Na1 Na2 120.7(3) . . ?
O9W Na1 Na2 42.1(3) . . ?
O37 Na1 Na2 81.4(3) . . ?
W6 Na1 Na2 154.3(2) . . ?
W2 Na1 Na2 145.6(2) . . ?
O9T Na1 W3 174.5(4) 1_655 . ?
O8W Na1 W3 82.8(3) . . ?
O67 Na1 W3 75.4(3) . . ?
O26 Na1 W3 91.7(3) . . ?
O23 Na1 W3 32.4(2) . . ?
O9W Na1 W3 109.2(3) . . ?
O37 Na1 W3 31.9(2) . . ?
W6 Na1 W3 92.59(14) . . ?
W2 Na1 W3 64.80(10) . . ?
Na2 Na1 W3 95.15(18) . . ?
O9T Na1 W7 127.8(3) 1_655 . ?
O8W Na1 W7 126.1(3) . . ?
O67 Na1 W7 32.0(2) . . ?
O26 Na1 W7 92.7(3) . . ?
O23 Na1 W7 75.6(3) . . ?
O9W Na1 W7 75.5(3) . . ?
O37 Na1 W7 34.4(2) . . ?
W6 Na1 W7 64.24(10) . . ?
W2 Na1 W7 92.41(14) . . ?
Na2 Na1 W7 99.87(19) . . ?
W3 Na1 W7 57.54(9) . . ?
O9W Na2 O16W 168.3(7) . . ?
O9W Na2 O17W 92.5(6) . 1_655 ?
O16W Na2 O17W 80.9(8) . 1_655 ?
O9W Na2 O5T 93.6(4) . 1_545 ?
O16W Na2 O5T 94.5(7) . 1_545 ?
O17W Na2 O5T 78.9(6) 1_655 1_545 ?
O9W Na2 O10W 76.0(4) . . ?
O16W Na2 O10W 112.9(7) . . ?
O17W Na2 O10W 160.5(7) 1_655 . ?
O5T Na2 O10W 86.0(4) 1_545 . ?
O9W Na2 O8W 89.5(4) . . ?
O16W Na2 O8W 82.4(7) . . ?
O17W Na2 O8W 101.0(6) 1_655 . ?
O5T Na2 O8W 176.9(5) 1_545 . ?
O10W Na2 O8W 94.6(4) . . ?
O9W Na2 O18W 152.7(7) . . ?
O16W Na2 O18W 37.3(8) . . ?
O17W Na2 O18W 113.3(8) 1_655 . ?
O5T Na2 O18W 83.3(7) 1_545 . ?
O10W Na2 O18W 76.7(6) . . ?
O8W Na2 O18W 93.9(7) . . ?
O9W Na2 Na6 93.6(4) . 1_655 ?
O16W Na2 Na6 86.2(7) . 1_655 ?
O17W Na2 Na6 33.4(6) 1_655 1_655 ?
O5T Na2 Na6 45.5(3) 1_545 1_655 ?
O10W Na2 Na6 130.2(4) . 1_655 ?
O8W Na2 Na6 134.4(4) . 1_655 ?
O18W Na2 Na6 103.1(6) . 1_655 ?
O9W Na2 Na1 47.1(3) . . ?
O16W Na2 Na1 125.0(7) . . ?
O17W Na2 Na1 103.5(5) 1_655 . ?
O5T Na2 Na1 140.5(3) 1_545 . ?
O10W Na2 Na1 80.4(3) . . ?
O8W Na2 Na1 42.6(3) . . ?
O18W Na2 Na1 128.2(6) . . ?
Na6 Na2 Na1 126.8(3) 1_655 . ?
O78 Na3 O7T 166.5(4) . 2 ?
O78 Na3 O7W 98.8(4) . . ?
O7T Na3 O7W 92.9(4) 2 . ?
O78 Na3 O4W 92.3(4) . . ?
O7T Na3 O4W 76.2(4) 2 . ?
O7W Na3 O4W 168.9(5) . . ?
O78 Na3 O4W 98.0(4) . 2 ?
O7T Na3 O4W 76.4(4) 2 2 ?
O7W Na3 O4W 84.6(4) . 2 ?
O4W Na3 O4W 94.8(4) . 2 ?
O78 Na3 O1W 89.8(4) . . ?
O7T Na3 O1W 94.9(4) 2 . ?
O7W Na3 O1W 98.9(4) . . ?
O4W Na3 O1W 80.2(4) . . ?
O4W Na3 O1W 170.9(5) 2 . ?
O78 Na3 Na3 97.6(3) . 2 ?
O7T Na3 Na3 69.6(3) 2 2 ?
O7W Na3 Na3 130.8(4) . 2 ?
O4W Na3 Na3 47.6(3) . 2 ?
O4W Na3 Na3 47.2(3) 2 2 ?
O1W Na3 Na3 127.3(4) . 2 ?
O78 Na3 W7 28.4(2) . . ?
O7T Na3 W7 138.3(3) 2 . ?
O7W Na3 W7 119.7(4) . . ?
O4W Na3 W7 70.9(3) . . ?
O4W Na3 W7 81.3(3) 2 . ?
O1W Na3 W7 103.9(3) . . ?
Na3 Na3 W7 69.36(19) 2 . ?
O3T Na4 O19W 88.4(7) 2_666 . ?
O3T Na4 O12W 175.7(5) 2_666 . ?
O19W Na4 O12W 90.3(7) . . ?
O3T Na4 O2T 90.3(4) 2_666 . ?
O19W Na4 O2T 86.4(7) . . ?
O12W Na4 O2T 85.6(4) . . ?
O3T Na4 O2W 77.2(4) 2_666 . ?
O19W Na4 O2W 165.3(7) . . ?
O12W Na4 O2W 104.3(4) . . ?
O2T Na4 O2W 96.3(4) . . ?
O3T Na4 O3W 86.3(4) 2_666 . ?
O19W Na4 O3W 92.3(7) . . ?
O12W Na4 O3W 97.8(5) . . ?
O2T Na4 O3W 176.4(5) . . ?
O2W Na4 O3W 84.2(5) . . ?
O3T Na4 O14W 97.6(6) 2_666 . ?
O19W Na4 O14W 17.7(7) . . ?
O12W Na4 O14W 82.3(6) . . ?
O2T Na4 O14W 101.4(6) . . ?
O2W Na4 O14W 161.6(6) . . ?
O3W Na4 O14W 77.9(6) . . ?
O3T Na4 Na8 131.9(4) 2_666 1_665 ?
O19W Na4 Na8 46.6(7) . 1_665 ?
O12W Na4 Na8 48.3(4) . 1_665 ?
O2T Na4 Na8 100.8(4) . 1_665 ?
O2W Na4 Na8 145.6(4) . 1_665 ?
O3W Na4 Na8 80.6(4) . 1_665 ?
O14W Na4 Na8 34.4(6) . 1_665 ?
O3T Na4 Na8 93.2(4) 2_666 2_666 ?
O19W Na4 Na8 54.7(7) . 2_666 ?
O12W Na4 Na8 89.3(4) . 2_666 ?
O2T Na4 Na8 140.7(4) . 2_666 ?
O2W Na4 Na8 122.6(4) . 2_666 ?
O3W Na4 Na8 38.5(4) . 2_666 ?
O14W Na4 Na8 39.4(6) . 2_666 ?
Na8 Na4 Na8 50.3(4) 1_665 2_666 ?
O17W Na5 O1T 87.4(7) . 2_566 ?
O17W Na5 O13 158.8(8) . . ?
O1T Na5 O13 113.5(6) 2_566 . ?
O17W Na5 O89 82.6(7) . . ?
O1T Na5 O89 137.6(6) 2_566 . ?
O13 Na5 O89 79.3(4) . . ?
O17W Na5 O38 97.2(7) . . ?
O1T Na5 O38 158.5(6) 2_566 . ?
O13 Na5 O38 64.9(4) . . ?
O89 Na5 O38 64.0(4) . . ?
O17W Na5 O19 116.8(7) . . ?
O1T Na5 O19 85.8(5) 2_566 . ?
O13 Na5 O19 63.8(4) . . ?
O89 Na5 O19 63.1(4) . . ?
O38 Na5 O19 110.3(5) . . ?
O17W Na5 O3W 93.5(7) . 2_666 ?
O1T Na5 O3W 72.1(5) 2_566 2_666 ?
O13 Na5 O3W 96.3(5) . 2_666 ?
O89 Na5 O3W 149.4(6) . 2_666 ?
O38 Na5 O3W 86.6(5) . 2_666 ?
O19 Na5 O3W 141.7(6) . 2_666 ?
O17W Na5 W3 130.3(7) . . ?
O1T Na5 W3 136.1(5) 2_566 . ?
O13 Na5 W3 33.9(3) . . ?
O89 Na5 W3 77.2(3) . . ?
O38 Na5 W3 33.3(3) . . ?
O19 Na5 W3 93.3(4) . . ?
O3W Na5 W3 82.5(4) 2_666 . ?
O17W Na5 Na6 31.6(6) . . ?
O1T Na5 Na6 108.9(5) 2_566 . ?
O13 Na5 Na6 133.5(5) . . ?
O89 Na5 Na6 82.4(4) . . ?
O38 Na5 Na6 68.6(4) . . ?
O19 Na5 Na6 139.0(5) . . ?
O3W Na5 Na6 78.8(5) 2_666 . ?
W3 Na5 Na6 100.3(4) . . ?
O17W Na5 W1 149.0(7) . . ?
O1T Na5 W1 93.0(4) 2_566 . ?
O13 Na5 W1 33.4(3) . . ?
O89 Na5 W1 76.3(3) . . ?
O38 Na5 W1 93.7(4) . . ?
O19 Na5 W1 32.6(2) . . ?
O3W Na5 W1 116.1(5) 2_666 . ?
W3 Na5 W1 66.6(2) . . ?
Na6 Na5 W1 157.0(4) . . ?
O17W Na5 W8 80.2(7) . . ?
O1T Na5 W8 164.4(5) 2_566 . ?
O13 Na5 W8 78.7(4) . . ?
O89 Na5 W8 31.6(2) . . ?
O38 Na5 W8 34.9(3) . . ?
O19 Na5 W8 91.4(4) . . ?
O3W Na5 W8 117.7(5) 2_666 . ?
W3 Na5 W8 59.36(18) . . ?
Na6 Na5 W8 64.1(3) . . ?
W1 Na5 W8 92.9(2) . . ?
O17W Na5 W9 92.9(7) . . ?
O1T Na5 W9 108.9(4) 2_566 . ?
O13 Na5 W9 77.3(3) . . ?
O89 Na5 W9 31.5(2) . . ?
O38 Na5 W9 91.9(4) . . ?
O19 Na5 W9 33.7(3) . . ?
O3W Na5 W9 173.5(5) 2_666 . ?
W3 Na5 W9 92.7(2) . . ?
Na6 Na5 W9 106.5(4) . . ?
W1 Na5 W9 57.67(17) . . ?
W8 Na5 W9 62.80(18) . . ?
O17W Na6 O13W 84.3(9) . . ?
O17W Na6 O11W 112.3(10) . . ?
O13W Na6 O11W 79.6(6) . . ?
O17W Na6 O8T 91.4(8) . . ?
O13W Na6 O8T 166.2(8) . . ?
O11W Na6 O8T 90.0(6) . . ?
O17W Na6 O5T 87.2(8) . 1_445 ?
O13W Na6 O5T 83.8(6) . 1_445 ?
O11W Na6 O5T 152.8(7) . 1_445 ?
O8T Na6 O5T 109.1(6) . 1_445 ?
O17W Na6 Na5 33.9(7) . . ?
O13W Na6 Na5 88.1(6) . . ?
O11W Na6 Na5 80.0(5) . . ?
O8T Na6 Na5 81.1(5) . . ?
O5T Na6 Na5 121.1(6) 1_445 . ?
O17W Na6 Na2 42.3(7) . 1_455 ?
O13W Na6 Na2 82.1(5) . 1_455 ?
O11W Na6 Na2 150.3(7) . 1_455 ?
O8T Na6 Na2 103.5(5) . 1_455 ?
O5T Na6 Na2 44.8(3) 1_445 1_455 ?
Na5 Na6 Na2 76.2(4) . 1_455 ?
O17W Na6 Na8 97.7(9) . . ?
O13W Na6 Na8 37.3(4) . . ?
O11W Na6 Na8 42.4(4) . . ?
O8T Na6 Na8 131.2(6) . . ?
O5T Na6 Na8 119.0(6) 1_445 . ?
Na5 Na6 Na8 80.7(4) . . ?
Na2 Na6 Na8 115.3(5) 1_455 . ?
O17W Na6 W5 108.9(8) . 1_445 ?
O13W Na6 W5 76.0(5) . 1_445 ?
O11W Na6 W5 129.1(6) . 1_445 ?
O8T Na6 W5 117.8(6) . 1_445 ?
O5T Na6 W5 24.2(3) 1_445 1_445 ?
Na5 Na6 W5 141.7(5) . 1_445 ?
Na2 Na6 W5 67.3(3) 1_455 1_445 ?
Na8 Na6 W5 104.2(4) . 1_445 ?
O17W Na6 W8 77.7(7) . . ?
O13W Na6 W8 143.6(7) . . ?
O11W Na6 W8 78.5(5) . . ?
O8T Na6 W8 23.0(3) . . ?
O5T Na6 W8 125.9(5) 1_445 . ?
Na5 Na6 W8 59.7(3) . . ?
Na2 Na6 W8 103.9(4) 1_455 . ?
Na8 Na6 W8 114.3(4) . . ?
W5 Na6 W8 139.8(4) 1_445 . ?
O17W Na6 Na7 107.6(8) . . ?
O13W Na6 Na7 156.2(6) . . ?
O11W Na6 Na7 112.9(6) . . ?
O8T Na6 Na7 37.3(3) . . ?
O5T Na6 Na7 76.5(4) 1_445 . ?
Na5 Na6 Na7 113.4(4) . . ?
Na2 Na6 Na7 93.0(3) 1_455 . ?
Na8 Na6 Na7 151.2(5) . . ?
W5 Na6 Na7 80.6(3) 1_445 . ?
W8 Na6 Na7 60.2(2) . . ?
O6W Na7 O6W 180.0(10) . 2_455 ?
O6W Na7 O1W 89.3(4) . . ?
O6W Na7 O1W 90.7(4) 2_455 . ?
O6W Na7 O1W 90.7(4) . 2_455 ?
O6W Na7 O1W 89.3(4) 2_455 2_455 ?
O1W Na7 O1W 180.0(4) . 2_455 ?
O6W Na7 O8T 99.1(4) . . ?
O6W Na7 O8T 80.9(4) 2_455 . ?
O1W Na7 O8T 81.0(3) . . ?
O1W Na7 O8T 99.0(3) 2_455 . ?
O6W Na7 O8T 80.9(4) . 2_455 ?
O6W Na7 O8T 99.1(4) 2_455 2_455 ?
O1W Na7 O8T 99.0(3) . 2_455 ?
O1W Na7 O8T 81.0(3) 2_455 2_455 ?
O8T Na7 O8T 180.0(4) . 2_455 ?
O6W Na7 Na6 59.1(4) . 2_455 ?
O6W Na7 Na6 120.9(4) 2_455 2_455 ?
O1W Na7 Na6 74.9(3) . 2_455 ?
O1W Na7 Na6 105.1(3) 2_455 2_455 ?
O8T Na7 Na6 147.1(3) . 2_455 ?
O8T Na7 Na6 32.9(3) 2_455 2_455 ?
O6W Na7 Na6 120.9(4) . . ?
O6W Na7 Na6 59.1(4) 2_455 . ?
O1W Na7 Na6 105.1(3) . . ?
O1W Na7 Na6 74.9(3) 2_455 . ?
O8T Na7 Na6 32.9(3) . . ?
O8T Na7 Na6 147.1(3) 2_455 . ?
Na6 Na7 Na6 180.000(1) 2_455 . ?
O14W Na8 O13W 94.3(10) 1_445 . ?
O14W Na8 O11W 178.5(11) 1_445 . ?
O13W Na8 O11W 84.2(7) . . ?
O14W Na8 O19W 15.3(9) 1_445 1_445 ?
O13W Na8 O19W 80.6(8) . 1_445 ?
O11W Na8 O19W 163.4(9) . 1_445 ?
O14W Na8 O3W 97.2(10) 1_445 2_666 ?
O13W Na8 O3W 87.0(7) . 2_666 ?
O11W Na8 O3W 82.7(6) . 2_666 ?
O19W Na8 O3W 103.2(9) 1_445 2_666 ?
O14W Na8 O14W 91.2(11) 1_445 2_666 ?
O13W Na8 O14W 166.4(10) . 2_666 ?
O11W Na8 O14W 90.2(8) . 2_666 ?
O19W Na8 O14W 106.1(11) 1_445 2_666 ?
O3W Na8 O14W 80.1(8) 2_666 2_666 ?
O14W Na8 O12W 94.6(9) 1_445 1_445 ?
O13W Na8 O12W 84.3(6) . 1_445 ?
O11W Na8 O12W 85.2(6) . 1_445 ?
O19W Na8 O12W 86.4(8) 1_445 1_445 ?
O3W Na8 O12W 165.7(8) 2_666 1_445 ?
O14W Na8 O12W 107.6(8) 2_666 1_445 ?
O14W Na8 Na8 53.3(8) 1_445 2_556 ?
O13W Na8 Na8 145.7(10) . 2_556 ?
O11W Na8 Na8 128.1(8) . 2_556 ?
O19W Na8 Na8 68.2(8) 1_445 2_556 ?
O3W Na8 Na8 86.5(7) 2_666 2_556 ?
O14W Na8 Na8 38.0(6) 2_666 2_556 ?
O12W Na8 Na8 107.0(8) 1_445 2_556 ?
O14W Na8 Na4 49.6(8) 1_445 1_445 ?
O13W Na8 Na4 94.9(6) . 1_445 ?
O11W Na8 Na4 130.4(7) . 1_445 ?
O19W Na8 Na4 45.1(6) 1_445 1_445 ?
O3W Na8 Na4 146.8(7) 2_666 1_445 ?
O14W Na8 Na4 98.1(7) 2_666 1_445 ?
O12W Na8 Na4 45.6(4) 1_445 1_445 ?
Na8 Na8 Na4 73.4(5) 2_556 1_445 ?
O14W Na8 Na6 135.5(10) 1_445 . ?
O13W Na8 Na6 41.2(5) . . ?
O11W Na8 Na6 43.1(5) . . ?
O19W Na8 Na6 121.8(8) 1_445 . ?
O3W Na8 Na6 81.0(6) 2_666 . ?
O14W Na8 Na6 131.4(8) 2_666 . ?
O12W Na8 Na6 85.0(5) 1_445 . ?
Na8 Na8 Na6 165.5(8) 2_556 . ?
Na4 Na8 Na6 121.1(5) 1_445 . ?
O14W Na8 Na4 94.7(9) 1_445 2_666 ?
O13W Na8 Na4 126.0(7) . 2_666 ?
O11W Na8 Na4 86.1(5) . 2_666 ?
O19W Na8 Na4 108.4(8) 1_445 2_666 ?
O3W Na8 Na4 39.1(4) 2_666 2_666 ?
O14W Na8 Na4 41.0(6) 2_666 2_666 ?
O12W Na8 Na4 147.4(6) 1_445 2_666 ?
Na8 Na8 Na4 56.3(5) 2_556 2_666 ?
Na4 Na8 Na4 129.7(4) 1_445 2_666 ?
Na6 Na8 Na4 109.2(4) . 2_666 ?
Ge1 O1GE W4 120.0(4) . . ?
Ge1 O1GE W9 121.9(5) . . ?
W4 O1GE W9 93.8(3) . . ?
Ge1 O1GE W1 125.8(4) . . ?
W4 O1GE W1 93.7(3) . . ?
W9 O1GE W1 93.6(3) . . ?
W1 O1T Na5 152.6(6) . 2_566 ?
Ge1 O2GE W5 120.8(4) . . ?
Ge1 O2GE W6 121.6(5) . . ?
W5 O2GE W6 93.4(3) . . ?
Ge1 O2GE W2 125.3(4) . . ?
W5 O2GE W2 94.2(3) . . ?
W6 O2GE W2 93.7(3) . . ?
W2 O2T Na4 136.8(5) . . ?
Ge1 O3GE W7 121.8(4) . . ?
Ge1 O3GE W8 120.3(4) . . ?
W7 O3GE W8 94.4(3) . . ?
Ge1 O3GE W3 124.5(5) . . ?
W7 O3GE W3 93.7(3) . . ?
W8 O3GE W3 94.6(3) . . ?
W3 O3T Na4 150.4(5) . 2_666 ?
Ge1 O4GE Zn1 120.1(5) . . ?
Ge1 O4GE Zn2 121.0(5) . 2_565 ?
Zn1 O4GE Zn2 96.5(4) . 2_565 ?
Ge1 O4GE Zn2 117.6(5) . . ?
Zn1 O4GE Zn2 97.9(4) . . ?
Zn2 O4GE Zn2 98.8(4) 2_565 . ?
W4 O4ZN Zn1 137.7(5) . . ?
W5 O5T Na2 141.3(5) . 1_565 ?
W5 O5T Na6 120.5(6) . 1_665 ?
Na2 O5T Na6 89.7(5) 1_565 1_665 ?
W5 O5ZN Zn2 138.3(5) . . ?
W6 O6ZN Zn1 128.6(5) . 2_565 ?
W6 O6ZN Zn2 134.9(5) . . ?
Zn1 O6ZN Zn2 94.3(4) 2_565 . ?
W7 O7A Zn1 128.9(5) . 2_565 ?
W7 O7A Zn2 132.4(5) . 2_565 ?
Zn1 O7A Zn2 95.9(4) 2_565 2_565 ?
W7 O7T Na3 149.7(5) . 2 ?
W8 O8A Zn2 140.2(5) . 2_565 ?
W8 O8T Na6 123.7(6) . . ?
W8 O8T Na7 125.8(5) . . ?
Na6 O8T Na7 109.8(5) . . ?
W9 O9T Na1 176.1(6) . 1_455 ?
W9 O9ZN Zn1 138.4(5) . . ?
W2 O12 W1 154.8(6) . . ?
W3 O13 W1 152.2(5) . . ?
W3 O13 Na5 100.4(5) . . ?
W1 O13 Na5 102.6(5) . . ?
W1 O14 W4 118.8(5) . . ?
W1 O19 W9 120.0(5) . . ?
W1 O19 Na5 100.4(5) . . ?
W9 O19 Na5 101.7(5) . . ?
W2 O23 W3 153.0(5) . . ?
W2 O23 Na1 101.9(4) . . ?
W3 O23 Na1 103.1(4) . . ?
W2 O25 W5 120.1(5) . . ?
W2 O26 W6 120.6(5) . . ?
W2 O26 Na1 103.0(4) . . ?
W6 O26 Na1 99.5(4) . . ?
W3 O37 W7 119.6(4) . . ?
W3 O37 Na1 102.4(4) . . ?
W7 O37 Na1 99.9(3) . . ?
W3 O38 W8 121.1(5) . . ?
W3 O38 Na5 99.1(5) . . ?
W8 O38 Na5 100.3(4) . . ?
W5 O45 W4 147.2(5) . . ?
W4 O49 W9 117.7(5) . . ?
W6 O56 W5 118.8(4) . . ?
W6 O67 W7 147.8(5) . . ?
W6 O67 Na1 104.4(4) . . ?
W7 O67 Na1 106.4(4) . . ?
W7 O78 W8 118.7(5) . . ?
W7 O78 Na3 116.0(4) . . ?
W8 O78 Na3 123.5(4) . . ?
W8 O89 W9 147.9(5) . . ?
W8 O89 Na5 104.4(4) . . ?
W9 O89 Na5 105.7(5) . . ?
Na7 O1W Na3 120.3(5) . . ?
Na8 O3W Na4 102.4(6) 2_666 . ?
Na8 O3W Na5 119.2(7) 2_666 2_666 ?
Na4 O3W Na5 117.3(6) . 2_666 ?
Na3 O4W Na3 85.2(4) . 2 ?
Na1 O8W Na2 92.5(4) . . ?
Na2 O9W Na1 90.7(4) . . ?
Na8 O11W Na6 94.6(7) . . ?
Na4 O12W Na8 86.0(5) . 1_665 ?
Na8 O13W Na6 101.4(7) . . ?
O19W O14W Na8 125(3) . 1_665 ?
O19W O14W Na8 144(3) . 2_666 ?
Na8 O14W Na8 88.8(11) 1_665 2_666 ?
O19W O14W Na4 67(3) . . ?
Na8 O14W Na4 95.9(10) 1_665 . ?
Na8 O14W Na4 99.6(9) 2_666 . ?
O18W O16W Na2 78.9(13) . . ?
Na6 O17W Na5 114.5(11) . . ?
Na6 O17W Na2 104.2(10) . 1_455 ?
Na5 O17W Na2 141.3(11) . 1_455 ?
O16W O18W O15W 105.8(18) . 1_545 ?
O16W O18W Na2 63.8(12) . . ?
O15W O18W Na2 149.4(15) 1_545 . ?
O14W O19W Na4 95(3) . . ?
O14W O19W Na8 40(2) . 1_665 ?
Na4 O19W Na8 88.3(9) . 1_665 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1T 1.707(10) . ?
W1 O14 1.858(9) . ?
W1 O19 1.892(9) . ?
W1 O12 1.918(9) . ?
W1 O13 1.951(9) . ?
W1 O1GE 2.378(9) . ?
W1 Na5 3.458(11) . ?
W2 O2T 1.712(9) . ?
W2 O25 1.865(9) . ?
W2 O26 1.909(9) . ?
W2 O12 1.910(9) . ?
W2 O23 1.920(9) . ?
W2 O2GE 2.372(9) . ?
W2 Na1 3.474(6) . ?
W3 O3T 1.708(9) . ?
W3 O38 1.882(9) . ?
W3 O37 1.894(9) . ?
W3 O13 1.919(9) . ?
W3 O23 1.927(9) . ?
W3 O3GE 2.367(9) . ?
W3 Na5 3.385(11) . ?
W3 Na1 3.506(6) . ?
W4 O4ZN 1.755(9) . ?
W4 O4T 1.766(10) . ?
W4 O45 1.924(9) . ?
W4 O49 1.935(9) . ?
W4 O14 2.088(9) . ?
W4 O1GE 2.279(9) . ?
W5 O5T 1.745(9) . ?
W5 O5ZN 1.770(9) . ?
W5 O45 1.920(9) . ?
W5 O56 1.975(9) . ?
W5 O25 2.069(9) . ?
W5 O2GE 2.285(9) . ?
W5 Na6 3.664(15) 1_665 ?
W6 O6T 1.709(10) . ?
W6 O6ZN 1.797(10) . ?
W6 O56 1.914(9) . ?
W6 O67 1.924(9) . ?
W6 O26 2.025(10) . ?
W6 O2GE 2.315(9) . ?
W6 Na1 3.470(6) . ?
W7 O7T 1.716(10) . ?
W7 O7A 1.809(9) . ?
W7 O78 1.917(9) . ?
W7 O67 1.956(9) . ?
W7 O37 2.029(9) . ?
W7 O3GE 2.281(9) . ?
W7 Na1 3.540(6) . ?
W7 Na3 3.621(6) . ?
W8 O8T 1.732(10) . ?
W8 O8A 1.746(9) . ?
W8 O89 1.913(9) . ?
W8 O78 1.988(9) . ?
W8 O38 2.053(9) . ?
W8 O3GE 2.299(9) . ?
W8 Na5 3.534(11) . ?
W8 Na6 3.682(14) . ?
W9 O9T 1.721(9) . ?
W9 O9ZN 1.779(10) . ?
W9 O89 1.950(9) . ?
W9 O49 1.960(10) . ?
W9 O19 2.035(10) . ?
W9 O1GE 2.288(9) . ?
W9 Na5 3.589(11) . ?
Ge1 O4GE 1.730(9) . ?
Ge1 O2GE 1.752(9) . ?
Ge1 O1GE 1.752(9) . ?
Ge1 O3GE 1.762(9) . ?
Zn1 O9ZN 2.050(9) . ?
Zn1 O1ZW 2.098(9) . ?
Zn1 O4GE 2.104(9) . ?
Zn1 O7A 2.108(9) 2_565 ?
Zn1 O4ZN 2.116(10) . ?
Zn1 O6ZN 2.133(10) 2_565 ?
Zn1 Zn2 3.144(2) 2_565 ?
Zn2 O8A 2.045(9) 2_565 ?
Zn2 O5ZN 2.052(10) . ?
Zn2 O4GE 2.110(9) 2_565 ?
Zn2 O4GE 2.114(9) . ?
Zn2 O6ZN 2.155(9) . ?
Zn2 O7A 2.176(9) 2_565 ?
Zn2 Zn1 3.144(2) 2_565 ?
Na1 O9T 2.357(11) 1_655 ?
Na1 O8W 2.361(12) . ?
Na1 O67 2.449(11) . ?
Na1 O26 2.504(11) . ?
Na1 O23 2.526(11) . ?
Na1 O9W 2.555(13) . ?
Na1 O37 2.573(10) . ?
Na1 Na2 3.485(9) . ?
Na2 O9W 2.338(12) . ?
Na2 O16W 2.37(3) . ?
Na2 O17W 2.39(2) 1_655 ?
Na2 O5T 2.429(12) 1_545 ?
Na2 O10W 2.436(12) . ?
Na2 O8W 2.463(13) . ?
Na2 O18W 2.59(3) . ?
Na2 Na6 3.444(16) 1_655 ?
Na3 O78 2.345(11) . ?
Na3 O7T 2.379(12) 2 ?
Na3 O7W 2.379(14) . ?
Na3 O4W 2.443(12) . ?
Na3 O4W 2.458(12) 2 ?
Na3 O1W 2.482(12) . ?
Na3 Na3 3.318(12) 2 ?
Na4 O3T 2.305(11) 2_666 ?
Na4 O19W 2.33(3) . ?
Na4 O12W 2.357(12) . ?
Na4 O2T 2.394(11) . ?
Na4 O2W 2.410(12) . ?
Na4 O3W 2.445(15) . ?
Na4 O14W 2.52(2) . ?
Na4 Na8 3.288(15) 1_665 ?
Na4 Na8 3.786(16) 2_666 ?
Na5 O17W 2.08(2) . ?
Na5 O1T 2.340(15) 2_566 ?
Na5 O13 2.463(14) . ?
Na5 O89 2.532(14) . ?
Na5 O38 2.533(14) . ?
Na5 O19 2.574(14) . ?
Na5 O3W 2.786(17) 2_666 ?
Na5 Na6 3.40(2) . ?
Na6 O17W 1.96(3) . ?
Na6 O13W 2.38(2) . ?
Na6 O11W 2.422(19) . ?
Na6 O8T 2.426(17) . ?
Na6 O5T 2.456(17) 1_445 ?
Na6 Na2 3.444(16) 1_455 ?
Na6 Na8 3.54(2) . ?
Na6 W5 3.664(14) 1_445 ?
Na6 Na7 4.205(15) . ?
Na7 O6W 2.265(12) . ?
Na7 O6W 2.265(12) 2_455 ?
Na7 O1W 2.401(10) . ?
Na7 O1W 2.401(10) 2_455 ?
Na7 O8T 2.710(10) . ?
Na7 O8T 2.710(10) 2_455 ?
Na7 Na6 4.205(15) 2_455 ?
Na8 O14W 1.87(3) 1_445 ?
Na8 O13W 2.186(19) . ?
Na8 O11W 2.390(19) . ?
Na8 O19W 2.39(3) 1_445 ?
Na8 O3W 2.41(2) 2_666 ?
Na8 O14W 2.44(3) 2_666 ?
Na8 O12W 2.463(18) 1_445 ?
Na8 Na8 3.04(3) 2_556 ?
Na8 Na4 3.288(15) 1_445 ?
Na8 Na4 3.786(16) 2_666 ?
O1T Na5 2.340(15) 2_566 ?
O3T Na4 2.305(11) 2_666 ?
O4GE Zn2 2.110(9) 2_565 ?
O5T Na2 2.429(12) 1_565 ?
O5T Na6 2.456(17) 1_665 ?
O6ZN Zn1 2.133(10) 2_565 ?
O7A Zn1 2.108(9) 2_565 ?
O7A Zn2 2.176(9) 2_565 ?
O7T Na3 2.379(12) 2 ?
O8A Zn2 2.045(9) 2_565 ?
O9T Na1 2.357(11) 1_455 ?
O3W Na8 2.41(2) 2_666 ?
O3W Na5 2.786(17) 2_666 ?
O4W Na3 2.458(12) 2 ?
O12W Na8 2.463(18) 1_665 ?
O14W O19W 0.77(3) . ?
O14W Na8 1.87(3) 1_665 ?
O14W Na8 2.44(3) 2_666 ?
O15W O18W 1.81(3) 1_565 ?
O16W O18W 1.60(3) . ?
O17W Na2 2.39(2) 1_455 ?
O18W O15W 1.81(3) 1_545 ?
O19W Na8 2.39(3) 1_665 ?
